A two-dimensional nematic phase of magnetic nanorods Kostyantyn Slyusarenko, Doru Constantin, Patrick Davidson To cite this version: Kostyantyn Slyusarenko, Doru Constantin, Patrick Davidson. A two-dimensional nematic phase of magnetic nanorods. Journal of Chemical Physics, American Institute of Physics (AIP), 2014, 140 (10), pp.104904. <10.1063/1.4867790>. <hal-00958646> HAL Id: hal-00958646 https://hal.archives-ouvertes.fr/hal-00958646 Submitted on 13 Mar 2014 HAL is a multi-disciplinary open access archive for the deposit and dissemination of scientific research documents, whether they are published or not. The documents may come from teaching and research institutions in France or abroad, or from public or private research centers. L’archive ouverte pluridisciplinaire HAL, est destin´ee au d´epˆot et `a la diffusion de documents scientifiques de niveau recherche, publi´es ou non, ´emanant des ´etablissements d’enseignement et de recherche fran¸cais ou ´etrangers, des laboratoires publics ou priv´es. A two-dimensional nematic phase of magnetic nanorodsa) Kostyantyn Slyusarenko,1 Doru Constantin,1, b) and Patrick Davidson1 Laboratoire de Physique des Solides, Universit´e Paris-Sud, CNRS, UMR 8502, 91405 Orsay, France. We report a hybrid mesophase consisting of magnetic nanorods confined between the non-ionic surfactant bilayers of a lamellar phase. The magnetic field-induced ordering of the nanorods was measured experimentally and modeled by a two-dimensional Onsager theory including the third virial coefficient. The nanorods are strongly confined in layers, with no orientational coupling from one layer to the next. At high volume concentration they exhibit spontaneous in-plane orientational ordering and form a stack of independent twodimensional nematic systems. This isotropic-nematic transition is first-order. PACS numbers: 82.70.Dd, 61.30.-v, 61.05.cf, 78.20.Fm I. • The nanorods have magnetic properties, hence their orientation can be controlled using an applied magnetic field. INTRODUCTION Ordered phases in reduced dimensions are fascinating systems, with physical properties that can be qualitatively different from those of their three-dimensional counterparts. One of the most (intuitively) straightforward examples would be the two-dimensional nematic phase, with quadrupolar orientational order but no positional order. This deceivingly simple system has been the topic of extensive theoretical1,2 and numerical3–5 work, with a particular emphasis on the first- or second-order character of the isotropic-nematic transition. There are however surprisingly few experimental realisations of such phases. The first qualitative observation involved rigid phospholipid tubules at the air-water interface6 . Similar results were obtained for LangmuirBlodgett films of nanorods7,8 , but the particles could only be observed after deposition on a substrate. Another strategy relies on inserting DNA molecules within stacks of neutral9,10 or charged11 lipid bilayers. These disordered mixtures were studied by X-ray scattering and the nematic phase was identified indirectly, by analyzing the shape of the DNA interaction peak. It is not clear whether these are purely two-dimensional phases or whether there is some interlayer coupling. We emphasize that the nematic order parameter was not measured in any of the systems above. In this paper, we present a system where rigid magnetic nanorods are inserted into a soft lamellar matrix of nonionic surfactant. The resulting phase has three key advantages: • It is easily aligned by thermal treatment, so that in the small-angle x-ray scattering (SAXS) images we can clearly discriminate between the direction of the smectic director and that in the plane of the layers. We can thus explore the anisotropy of the phase. a) Originally published in J. Chem. Phys. 140(10), 104904 (2014); http://dx.doi.org/10.1063/1.4867790 b) Electronic mail: [email protected] • When the phase is aligned in homeotropic anchoring, we can perform optical birefringence measurements (in particular under magnetic field), which yield a completely independent estimate of the orientational order of the particles. The formulation of the phase12 and its structural study13 have already been presented. Here, we are concerned with the orientational order of the particles under magnetic field, that we describe using an Onsager-type model (up to the third virial coefficient), accounting for the electrostatic effects and for an applied magnetic field. We conclusively demonstrate a first-order phase transition between two-dimensional isotropic and nematic phases, settling a long-standing debate in the theoretical and numerical literature3–5,14,15 . II. MODEL AND ANALYSIS The nanorods can be seen as parallelepipeds, with dimensions L × W × H and volume V = LW H. They bear a permanent magnetic moment µ along their long axis and exhibit negative susceptibility anisotropy ∆χ = χk − χ⊥ < 0. For simplicity, we will describe them in thepfollowing as cylinders of length L and diameter D = 4W H/π. The particle orientation is quantified by the distribution f (Ω), such that a fraction f (Ω)dΩ of particles have their long axes e within the solid angle element dΩ around direction Ω. Our main result concerns the orientational distribution of the particles under confinement, but we start the discussion with their behavior in aqueous solution, a configuration that we will use as reference. In isotropic solution at a volume concentration φ and in the presence of a magnetic field (taken along the polar axis, B = B zˆ), f (Ω) can be described by an extended 2 Onsager model16,17 : 1 f (Ω) = exp KB cos θ + JB 2 P2 (cos θ) A Z 32 φ ′ ′ ′ − |sin γ(Ω, Ω )| f (Ω )dΩ π φ∗ (1) , where P2 is the Legendre with K = kBµT and J = 3µ∆χV 0 kB T polynomial of the second order, γ is the angle between two rods oriented along directions Ω = (θ, ϕ) and Ω′ = (θ′ , ϕ′ ), while φ∗ = 4D2 L (D + X)(L + X)2 (2) is the spinodal concentration (above which the isotropic state is absolutely unstable), X is an effective length describing the electrostatic interaction between rods16 (X = (ln A′ + γ + ln 2 − 0.5)/κ, with A′ the amplitude of the electrostatic interaction, γ ≈ 0.577 Euler’s constant, and κ−1 the Debye screening R length), and A is a normalization constant imposing f (Ω)dΩ = 1. Equation (1) is implicit in f (Ω) and must be solved numerically. The resulting order parameter S is used to fit the experimental data. When the particles are confined in the lamellar phase (with interlayer spacing d), we consider that within the same layer they have the same effective interaction as in solution so we model them using the 2D analogue of Equation (1), but this time the polar axis is along the director zˆkn and the magnetic field is applied in the plane of the layers B⊥n : 1 f (ϕ) = exp KB cos ϕ + JB 2 P2 (cos ϕ) A Z 2π k2 (ϕ, ϕ′ )f (ϕ′ )dϕ′ −η 0 (3) Z 2π Z 2π 2 ′ ′′ ′ ′′ ′ ′′ −η k3 (ϕ, ϕ , ϕ )f (ϕ )f (ϕ )dϕ dϕ 0 0 Z 2π M 2 ′ ′ ′ cos (ϕ − ϕ )f (ϕ )dϕ , +η kB T 0 where the in-plane angle ϕ is measured with respect to the orientation of the magnetic field and η, 4φd(L + X)(D + X) η= , πD2 L is the effective surface fraction. By using D, we implicitly consider that the particles can rotate freely along their long axis, as in the isotropic solution. If they were to adopt a particular configuration, for instance with the largest face (L × W ) in contact with the surfactant bilayer, the values of X and η would be slightly changed. However, we have no experimental evidence for or against this assertion and, for simplicity’s sake, we conserve the “cylindrical” model used above. In (3) the third and fourth terms on the right-hand side describe the second and third virial coefficients of the Onsager interaction. The coefficient k2 (ϕ, ϕ′ ) has an analytical form, 1 | sin(ϕ − ϕ′ )| + 2[1 + | cos(ϕ − ϕ′ )|], k2 (ϕ, ϕ′ ) = λ + λ L+X is the effective aspect ratio, and D+X the coefficient k3 (ϕ, ϕ′ , ϕ′′ ) is calculated numerically4 . Note that Onsager’s argument for neglecting higher-order virial terms does not apply in 2D4,18 , especially for rods of moderate aspect ratio (such as those used in our experiments). We therefore kept the third term in the virial expansion. As presented so far, the 2D model considers that particles in the same plane interact by the effective hard-core model measured in solution, while particles in different layers do not interact at all. This latter feature is indispensable for having a true 2D phase, so it should be thoroughly checked. That is why we added in (3) a possible orientational coupling19 between the nanorods in neighboring layers, described by the last term (with M the coupling amplitude). Below, we discuss possible physical origins for such a coupling, estimate its strength and show that it is negligible. where λ = A. X-ray scattering The X-ray scattering form factor of an individual particle is: F (q, β, L, D) = F0 sinc qL cos β 2 J1 (qD/2 sin β) qD/2 sin β (4) where β is the angle between the long axis of the rod e and the scattering vector q: cos β = cos θ sin ψ + sin θ cos ψ cos ϕ (see also Figure 1). For a monodisperse population, the scattering signal is given by20 : Z 2π Z π/2 I(q, ψ) = 2 dϕ fMS (θ)F 2 (q, β) sin(θ)dθ (5) 0 0 while in the general (polydisperse) case Equation (5) must be averaged over a radius distribution g(D) (the polydispersity in the length L does not contribute over the available q-range.) In (5) we approximate the orientational distribution of the rods by the analytical MaierSaupe form: fMS (Ω) = exp(m cos2 θ) Z (6) where Z is a normalization constant and fitted the data with only one parameter m. The order parameter S can be expressed analytically as a function of m. 3 0.1 0.5% 1.5% 3.5% 0.0 S(B) -0.1 -0.2 -0.3 -0.4 FIG. 1. Experimental geometry. The scattering object is a rod with orientation e given by the polar angle θ (measured with respect to the nematic director nkˆ z ) and the azimuthal angle ϕ. The incident beam is along the yˆ axis. The detector records in the (x, z) plane (normal to the incident beam) the scattered intensity I(q, ψ) given by Equation (5) B. Optical birefringence The birefringence of the samples can generally be expressed as: ∆n = ∆nsat S(B)φ (7) where the field-dependent order parameter S(B) is the uniaxial one S for the case of water suspensions and the in-plane component 23 P of the biaxial order when the particles are confined within the lamellar matrix. ∆nsat is the specific birefringence, depending on the geometry of the particles and on their dielectric permittivity tensor. III. RESULTS AND DISCUSSION From electron microscopy and X-ray diffraction measurements, the average particle dimensions are: L = 315 nm × W = 38 nm × H = 18 nm , -0.5 0 800 1000 1200 1400 1600 The order parameter is then computed over the distribution f (θ) determined from the complete model (1) as a function of B and φ, yielding estimates for the material constants K and J. The spinodal concentration φ∗ = 7.1% was estimated from the independent measurement of the phase diagram of the aqueous suspension in zero field: φ∗ ≈ 0.95φ3D N , where φ3D is the volume concentration of the nematic N phase at coexistence (in aqueous solution). From (2) we then obtain X = 72 nm. We also measured the birefringence ∆n(B) of the solutions (Figure 3) and fitted it to Equation (7), which involves the additional constant ∆nsat . Finally, we obtain the material constants: K = 8.2 ± 0.5 T−1 and the relative polydispersity is of the order of 0.3 . They correspond to cylinders with a diameter D = p 4W H/π = 29.5 nm. Under a magnetic field B, aqueous solutions of nanoparticles become uniaxial, with a director nkB and an order parameter S that can be positive or negative, depending on the field amplitude17 . From the SAXS images we determined the order parameter S(B) as a function of the field (Figure 2) by fitting the data to Equation (5) and using for the orientation distribution the Maier-Saupe form (6). The polydispersity g(D) is estimated from the scattering spectrum of a dilute suspension in the absence of the field. 600 FIG. 2. Order parameter S(B) (determined from the SAXS images) for the aqueous suspensions of nanorods at various concentrations φ (symbols). The curves are fits derived from Equation (1) with parameter values (9) (8) In solution 400 B (mT) 13 A. 200 −2 J = −13.8 ± 1 T ∆nsat = 0.8 φ∗ = 7.1% ⇒ X = 72 nm (9a) (9b) (9c) (9d) that we use alongside the particle dimensions (8) to study the hybrid system (particles inserted in the lamellar matrix). B. In the lamellar phase The SAXS measurements can be performed in either homeotropic or planar anchoring, giving access to both S and P , but the optical birefringence can only be determined in the homeotropic configuration (sensitive to P ). 4 0.002 0.5 % 1.5 % 3.5 % 0.0015 0.000 Birefringence Birefringence -0.002 -0.004 -0.006 0.5% 1.5% 3.5% -0.008 -0.010 0.0010 0.0005 0.0000 -0.012 0 200 400 600 0 800 100 B (mT) In the planar configuration, with B = 0, for φ = 0.5%, 1.5%, and 3.5% we obtained S = −0.44, −0.46, and −0.47, respectively, very close to the perfect confinement limit S = −0.5. We conclude that, even in the absence of the field, the particles are practically contained within the plane of the layers (and the optical axis is along n). If we now apply a field B⊥n the system becomes biaxial, with a second order parameter P . In the following we treat the system as purely twodimensional, with S = −0.5. The particle population is then completely described by the orientation distribution f (ϕ), determined from the model (3) as a function of B, M , and φ. The material constants are those measured in aqueous solution (9), the periodicity of the lamellar phase d = 45 nm,13 and M is the sole fitting parameter. 300 FIG. 4. Birefringence ∆n(B) of the suspensions of nanorods in lamellar phase at various concentrations φ (symbols). The curves are fits derived from Equations (7) (with S(B) replaced by (2/3)P (B)) and (3) with the material parameters in (9), d = 45 nm, and M = −3 kB T . 0.05 P FIG. 3. Birefringence ∆n(B) of the aqueous suspensions of nanorods at various concentrations φ (symbols). The curves are fits derived from Equations (7) and (1) with parameter values (9) 200 B (mT) 0.00 0.5 % 1.5 % 3.5 % -0.05 0 100 200 300 B (mT) 1. Isotropic two-dimensional phase We describe the birefringence ∆n(B) using Equation (7) (with S(B) replaced by (2/3)P (B)) coupled with (3). The simultaneous fit of the three curves yields M = (−3 ± 3) kB T see Figure 4, and the resulting order parameter is compared to that measured by SAXS in Figure 5. The M values for the individual fits at 1.5 and 3.5 % are shown in Figure 7. At 0.5 % the uncertainty on M is very large, so we excluded this point from the analysis. 2. Nematic two-dimensional phase The most concentrated system, with φ = 8 vol % in the lamellar phase is a biaxial nematic, with a spontaneous FIG. 5. Second order parameter P (B) (determined from the SAXS images) of the suspensions of nanorods in lamellar phase at various concentrations φ (symbols). The curves are fits derived from Equation (3) with the material parameters in (9), d = 45 nm, and M = −3 kB T . second order parameter P . It can thus be seen as a stack of two-dimensional nematic layers. To measure P we applied a small magnetic field of 30 mT in the plane of the layers to orient all nematic domains along the field, and measured the dependence of the x-ray scattering intensity I on ψ. Fitting I(ψ) by the Leadbetter method21 , which takes into account the interaction between nanorods (and is more appropriate at high concentration than the model (5)), we obtained P = 0.51. Both in aqueous solution and in the lamellar phase 5 2 0 -2 M ( kBT ) the isotropic-nematic transition is first-order, as the two phases can coexist over a certain concentration range. By preparing several samples within this domain and estimating the fraction occupied by each phase we determine the nematic concentration at coexistence φ3D N (in the aqueous solution) and φN (for the two-dimensional nematic). In our system, these two distinct parameters happen to have the same numerical value, 7.5±0.5 vol %. In the lamellar phase, the isotropic-nematic coexistence range is approximately φ = 4.5 − 7.5 vol %, corresponding to η = 0.38 − 0.6213 . A sample at coexistence, with φ = 6.6 vol %, i.e. η = 0.54, is shown in Figure 6. The interface is not sharply defined, mainly due to the presence of the lamellar defects which create arbitrarily shaped domains of the two phases. -4 -6 -8 0 1 2 3 4 5 6 7 8 9 10 φ(%) I/Lα FIG. 7. Best estimate of M for various concentrations φ. For φ = 1.5 and 3.5 % we used the birefringence data (Figure 4). The two high-concentration points are obtained from the transition concentration and from P (φ = 0.08) (see text). N/Lα FIG. 6. Sample at coexistence (φ = 6.6 vol %, η = 0.54). The dashed line (with a greyed uncertain area) delimits the 2D isotropic phase I/Lα (upper left) from the 2D nematic phase N/Lα (lower right). The width of the capillary is 1 mm. The two-dimensional model (3) does indeed predict a first-order isotropic-nematic transition, with a φN that corresponds to the experimental one (φexp = 7.5 ± N 0.5 vol %) for M = (0.5 ± 0.5) kB T . For our most concentrated sample, with φ = 8 vol %, the same model reproduces the order parameter P = 0.51 for M = (0.07 ± 0.01) kB T . These two values correspond to the high-concentration points in Figure 7. 3. Coupling The coupling coefficient M is not significantly different from zero: at low concentration (in the two-dimensional isotropic phase) M = (−3±3) kB T from the birefringence data and at high concentration (in the two-dimensional nematic phase) M = (0.5 ± 0.5) kB T from the transition concentration and M = (0.07 ± 0.01) kB T from P (φ = 0.08). We conclude that, within the experimental precision, the orientation of particles in different layers is uncoupled, see Figure 7. Is this result in agreement with the theoretical estimations? The main difference between the particles in lamellar phase and those in isotropic solution is that the former are constrained to lie in parallel planes, and thus can more easily become parallel. Magnetic and electrostatic interaction might then be stronger than in three dimensions. We estimate their amplitude in the twodimensional nematic phase, at φ = 8 vol %: The magnetic interaction between the permanent dipole moments of the particles Wdd favors an antiparallel orientation and its magnitude is: Wdd µ0 µ2 µ0 K 2 kB T φ ≈ ≈ = 6 · 10−6 , kB T 4πr3 kB T 4πLDH where r is an average interparticle distance. The electrostatic twist energy22 per molecule Wtw (which favors a perpendicular orientation) is given by23 : Z Z Wtw ηhtw = ktw (ϕ, ϕ′ )f (ϕ)f (ϕ′ )dϕdϕ′ , (10) kB T 2 where htw = (κX)−1 . The coefficient ktw (ϕ, ϕ′ ) is: 1 [−| sin(ϕ − ϕ′ )| ln | sin(ϕ − ϕ′ )| ktw (ϕ, ϕ′ ) = λ + λ − α| sin(ϕ − ϕ′ )|], with α=− RR | sin(ϕ − ϕ′ )| ln | sin(ϕ − ϕ′ )|dϕdϕ′ RR ≈ 0.3065. | sin(ϕ − ϕ′ )|dϕdϕ′ The main uncertainty is in evaluating the Debye length: κ−1 = 2−14 nm, where the lower value was measured in a different goethite batch17 and the higher one corresponds 6 to an ionic strength of 1 mM (the minimum possible at pH = 3). We then have Wtw ≈ (4 − 25) · 10−3 kB T . Both effects are therefore negligible compared to the thermal energy, in agreement with our experimental findings. IV. CONCLUSION We formulated stable anisotropic materials where goethite nanorods are confined between the bilayers of a soft lamellar phase. The nanorods form a nematic system with director along the director of the lamellar phase and a negative order parameter S≤ − 0.45 (to be compared with S = −0.5 for perfect confinement). At low volume concentration φ < 7.5 vol %, the system is uniaxial in the absence of a magnetic field and forms a two-dimensional isotropic phase. Under a small magnetic field (0 < B < 350 mT) parallel to the layers, the distribution of the nanorods acquires a biaxial character (the long axis is preferentially oriented along the field), with a low order parameter P (P ≤ 0.05 for φ = 3.5 vol %). At higher concentration φ ≥ 7.5vol % the biaxial order is spontaneous, yielding a two-dimensional nematic phase in the plane perpendicular to n, with an order parameter P ≃ 0.51. We modelled the magnetic field-induced ordering of the nanorods P (B) by a two-dimensional Onsager theory and obtained good agreement with the experiment. In the simulation we took into account the magnetic properties of the nanorods and the effect of the electrostatic interaction and expanded the free energy to the third virial coefficient. We also included a possible orientational coupling M between nanorods in neighboring layers. We conclude that M is not significantly different from zero (and, at any rate, much smaller than kB T ) and that the phase is a stack of isolated layers. The particles can be modelled as rigid rectangles with aspect ratio 3.8; at low concentration they exhibit a twodimensional isotropic phase which (on increasing the concentration) undergoes a first-order phase transition to a two-dimensional nematic phase with an order parameter P ∼ 0.5. This result is in very good agreement with numerical simulations4,24 . In our analysis, we chose a particular effective shape (rigid rectangles) for the particles, mainly due to its tractability (very important for including the third virial coefficient). Other choices can lead to a different phase diagram, in particular to a second-order phase transition25 , in contrast with the experimental findings. We also ignored the effect of polydispersity, which could have profound consequences26 . Hopefully, our experimental results will motivate further theoretical and numerical research in the field of two-dimensional ordered phases. ACKNOWLEDGMENTS We acknowledge support from the Triangle de la Physique (project 2011-083T). The ESRF is acknowledged for the provision of beamtime (experiment SC2393, ID02 beamline). The authors thank C. Chan´eac for the goethite suspension, P. Boesecke, M. Imp´eror, A. Poulos, and B. Pansu for assistance with the SAXS experiments, J. Andrieu for performing some of the optical birefringence measurements and L. Navailles for stimulating discussions. 1 Z. Y. Chen, “Continuous isotropic-nematic transition of partially flexible polymers in two dimensions,” Phys. Rev. Lett., 71, 93 (1993). 2 P. van der Schoot, “Nematics of linear assemblies in two dimensions,” J. Chem. Phys., 106, 2355 (1997). 3 M. Cosentino Lagomarsino, M. Dogterom, and M. Dijkstra, “Isotropic-nematic transition of long, thin, hard spherocylinders confined in a quasi-two-dimensional planar geometry,” The Journal of Chemical Physics, 119, 3535 (2003). 4 Y. Mart´ ınez-Rat´ on, E. Velasco, and L. Mederos, “Orientational ordering in hard rectangles: the role of the three body correlations,” J. Chem. Phys., 125, 014501 (2006). 5 R. L. C. Vink, “Liquid crystals in two dimensions: First-order phase transitions and nonuniversal critical behavior,” Phys. Rev. Lett., 98, 217801 (2007). 6 M. R. Fisch and C. Rosenblatt, “Observation of quasi twodimensional nematic order in a system of rigid rods,” J. Phys. II France, 4, 103 (1994). 7 F. Kim, S. Kwan, J. Akana, and P. D. Yang, “Langmuir-Blodgett nanorod assembly,” Journal of the American Chemical Society, 123, 4360 (2001). 8 L. S. Li and A. P. Alivisatos, “Semiconductor nanorod liquid crystals and their assembly on a substrate,” Advanced Materials, 15, 408 (2003). 9 T. Pott and D. Roux, “DNA intercalation in neutral multilamellar membranes,” FEBS Letters, 511, 150 (2002). 10 T. Pott, A. Colin, L. Navailles, and D. Roux, “DNA intercalation in neutral multilamellar membranes: Experiments and theory,” Interface Science, 11, 249 (2003). 11 N. F. Bouxsein, C. Leal, C. S. McAllister, K. K. Ewert, Y. Li, C. E. Samuel, and C. R. Safinya, “Two-dimensional packing of short DNA with nonpairing overhangs in cationic liposomeDNA complexes: From Onsager nematics to columnar nematics with finite-length columns,” Journal of the American Chemical Society, 133, 7585 (2011). 12 K. B´ eneut, D. Constantin, P. Davidson, A. Dessombz, and C. Chan´ eac, “Magnetic nanorods confined in a lamellar lyotropic phase,” Langmuir, 24, 8205 (2008). 13 D. Constantin, P. Davidson, and C. Chan´ eac, “Lyotropic lamellar phase doped with a nematic phase of magnetic nanorods,” Langmuir, 26, 4586 (2010). 14 A. C. D. van Enter and S. B. Shlosman, “First-order transitions for n-vector models in two and more dimensions: Rigorous proof,” Phys. Rev. Lett., 89, 285702 (2002). 15 N. G. Almarza, C. Mart´ ın, and E. Lomba, “Phase behavior of the confined Lebwohl-Lasher model,” Phys. Rev. E, 82, 011140 (2010). 16 G. J. Vroege and H. N. W. Lekkerkerker, “Phase transitions in lyotropic colloidal and polymer liquid crystals,” Rep. Prog. Phys., 55, 1241 (1992). 17 B. J. Lemaire, P. Davidson, J. Ferr´ e, J. P. Jamet, D. Petermann, P. Panine, I. Dozov, and J. P. Jolivet, “Physical properties of aqueous suspensions of goethite (α-FeOOH) nanorods; Part I: In the isotropic phase,” Eur. Phys. J. E, 13, 291 (2004). 18 J. P. Straley, “Liquid crystals in two dimensions,” Phys. Rev. A, 4, 675 (1971). 7 19 In principle, one could also have a positional coupling between layers. We do not include this type of term, because here we concentrate on the orientational order and because an extensive X-ray scattering investigation showed no characteristic sign (peak with qz 6= 0 and qr 6= 0) of such coupling. 20 B. J. Lemaire, P. Panine, J. C. P. Gabriel, and P. Davidson, “The measurement by SAXS of the nematic order parameter of laponite gels,” Europhys. Lett., 59, 55 (2002). 21 A. J. Leadbetter and E. K. Norris, “Distribution functions in three liquid crystals from X-ray diffraction measurements,” Molecular Physics, 38, 669 (1979). 22 This is simply the repulsion between identical and uniformly charged rods placed on top of each other in parallel planes. 23 A. Stroobants, H. N. W. Lekkerkerker, and T. Odijk, “Effect of electrostatic interaction on the liquid crystal phase transition in solutions of rodlike polyelectrolytes,” Macromolecules, 19, 2232 (1986). 24 J. A. Cuesta and D. Frenkel, “Monte Carlo simulation of twodimensional hard ellipses,” Phys. Rev. A, 42, 2126 (1990). 25 Y. Mart´ ınez-Rat´ on, E. Velasco, and L. Mederos, “Effect of particle geometry on phase transitions in two-dimensional liquid crystals,” The Journal of Chemical Physics, 122, 064903 (2005). 26 Y. Mart´ ınez-Rat´ on, “Phase behaviour of mixtures of hard ellipses: a scaled particle density functional study,” Liquid Crystals, 38, 697 (2011). 27 P. Palffy-Muhoray and G. L. Hoatson, “Mean-field theory of binary mixtures of nematic liquid crystals consisting of biaxial molecules,” Phys. Rev. A, 44, 5052 (1991), in our notation symbols S and Q are swapped with respect to this reference. ORDER PARAMETER The order parameter tensor Q of the phase describes the distribution of the particle direction e: Qαβ = 1 − δαβ ) (where the average h·i is taken over the distribution f (Ω)) and can be written in the principal axis frame as (Palffy-Muhoray and Hoatson 27 , Eq. 7): 2 (3eα eβ Qαβ − 21 (S − P ) 0 0 = 0 − 12 (S + P ) 0 0 0 S (11) In spherical coordinates, with the polar axis along zˆ, the values of P and S are related to the distribution function f (θ, ϕ) via: ZZ 1 3 f (θ, ϕ) sin θ cos2 θ dθdϕ − 2 2 ZZ 3 P = f (θ, ϕ) sin3 θ cos(2ϕ) dθdϕ 2 S= (12) For a uniaxial system the distribution f depends only on the polar angle, f (Ω) = f (θ), P R= 0 and S is defined via the simplified formula: S = 23 f (θ) sin θ cos2 θ dθ − 1 2 . In the “complete confinement” case (relevant for the 1 lamellar system), f (Ω) R = δ(θ − π/2)f (ϕ), S = − 2 , and 3 P reduces to: P = 2 f (ϕ) cos(2ϕ) dϕ.
© Copyright 2021 ExpyDoc